Optical and structural characterization
of oleic acid-stabilized CdTe nanocrystals
for solution thin film processing
Claudio Davet Gutiérrez-Lazos1, Mauricio Ortega-López2,
Manuel A. Pérez-Guzmán3, A. Mauricio Espinoza-Rivas2,
Francisco Solís-Pomar1, Rebeca Ortega-Amaya2,
L. Gerardo Silva-Vidaurri1, Virginia C. Castro-Peña1
and Eduardo Pérez-Tijerina*1,§
Full Research PaperOpen Access
1Centro de Investigación en Ciencias Físico Matemáticas, Facultad de Ciencias Físico Matemáticas, Universidad Autónoma de Nuevo León, Av. Universidad s/n. Ciudad Universitaria, 66451 San Nicolás de los Garza, Nuevo León, México, 2Sección de Electrónica del Estado Sólido, Centro de Investigación y de Estudios Avanzados del Instituto Politécnico Nacional, Av. Instituto Politécnico Nacional 2508, Col. San Pedro Zacatenco, 07360 México, D. F., México and
3Programa de Doctorado en Nanociencias y Nanotecnología, Centro de Investigación y de Estudios Avanzados del Instituto Politécnico Nacional, Av. Instituto Politécnico Nacional 2508, Col. San Pedro Zacatenco, 07360 México, D. F., México
Eduardo Pérez-Tijerina* - Eduardo.firstname.lastname@example.org * Corresponding author
§ Tel. and Fax: +52 (81) 1340 4000 ext. 7106.
cadmium telluride; Raman spectroscopy; semiconductor nanocrystals; transmission electron microscopy; X-ray diffraction
Beilstein J. Nanotechnol.2014,5, 881–886. doi:10.3762/bjnano.5.100
Received: 11 February 2014 Accepted: 20 May 2014 Published: 20 June 2014
Associate Editor: J. J. Schneider
© 2014 Gutiérrez-Lazos et al; licensee Beilstein-Institut. License and terms: see end of document.
LO modes of cubic CdTe nanocrystals, respectively. Additional peaks located in the 222 to 324 cm−1 range, agree fairly well with the wavenumbers reported for TO modes of octahedral Cd3P2.
Figure 1: a) TEM micrograph of CdTe nanocrystals, the inset shows the indexed electron diffraction pattern, b) TEM image of CdTe nanocrystals used to determinate the lattice parameter. The inset shows the 3.23 Å (200) lattice parameter.
Currently colloidal chemistry is a promising technique in ma-terials science research due to its simplicity, low cost, and its capability to process nearly-monodisperse nanocrystals of a variety of semiconductor materials at low temperatures and using non sophisticated equipments [1,2]. It has been exten-sively used to prepare binary [3-5], ternary [6-8] and quater-nary [9,10] semiconductors for applications in quantum effect based devices  such as light emitting diodes , biola-beling , thermoelectric generators  and thin film solar cells . In solar cell technology, colloidal nanocrystals hold promise for producing cheap solar cells with improved conver-sion efficiency by using quantum effects such as multiple exciton generation . In the last years, nanostructured semi-conductors have proved to be useful as raw material for solu-tion-processable electronic technologies. The capping of semi-conductor nanocrystals by organic ligands, provides the control of composition, size, shape and crystal structure, which make them very attractive in this technological area. Thin films depo-sition techniques such as drop-casting , screen printing , and ink jet printing , are currently used to fabricate elec-tronic devices on great variety of substrates, either rigid or flex-ible, looking for preserve their size effects [20-22]. All of these techniques need ink-like stable dispersions comprising function-alized nanomaterials dispersed in a convenient solvent. Drop-casting offers a cost efficient production of photovoltaic semi-conductor thin films. Nevertheless, depending on the dispersion chemistry and on the required thin film optoelectronic prop-erties, post-deposition complex processes are needed. Guo et al.  deposited CuInSe2 (CIS) thin films for solar cells starting from oleylamine-stabilized CIS nanocrystals. An additional annealing at 500 °C was needed to obtain suitable CIS films for
photovoltaic applications. Jasieniak et al.  deposited photo-voltaic cadmium telluride (CdTe) thin films by using pyridine-capped CdTe nanocrystals. In their approach, CdTe nanocrys-tals were deposited from solution by a layer-by-layer process with subsequent annealing per layer at 300, 350 and 400 °C. On the other hand, oleic acid is a green organic ligand, which has been successfully used in preparing a great variety of colloidal materials [15,25,26], including CdTe quantum dots [27-29].
This work presents our early results on the elaboration of CdTe-based inks for potential uses in solution-processable thin film solar cells. The CdTe-NC were prepared by colloidal chemistry using an organic–inorganic reaction . The product comprised toluene-dispersed oleic acid-stabilized CdTe-NC and cadmium phosphide (Cd3P2) as a secondary phase. Oleic acid was chosen because it enabled us to manipulate the CdTe nanocrystals under ambient conditions, and to use them to deposit CdTe thin films that were free of cadmium tellurate or tellurium oxide. The CdTe nanocrystals and thin films were characterized by TEM, X-ray diffraction, UV–vis spectroscopy and Raman spectroscopy.
Results and Discussion
Beilstein J. Nanotechnol.2014,5, 881–886.
electron diffraction pattern (inset Figure 1a), indicated the face-centered cubic phase for CdTe as reported by Talapin et al. . The electron diffraction pattern was indexed following the method reported elsewhere . In addition, an extra phase was disclosed; it was attributed to the Cd3P2 impurity phase, which crystalizes in the octahedral structure. The above described features could be corroborated by XRD and Raman spec-troscopy (see below).
Figure 2 shows a CdTe deposition with and without UV illumi-nation. We further note that the nanocrystal luminescence under ambient conditions is preserved.
Figure 2: CdTe deposition with and without UV illumination under ambient conditions.
X-ray diffraction analysis
The structural properties of the prepared samples were evalu-ated by XRD and Raman spectroscopy, using CdTe thin films deposited on glass substrates (see Figure 2). As mentioned above, XRD and Raman measurements corroborated the phase composition of the colloids. Figure 3 shows the X-ray diffrac-tion patterns of deposited CdTe-NC at concentradiffrac-tions of 2.24 and 0.45 mmol trioctylphosphine (TOP), respectively. The diffraction patterns display the typical low intensity and broad peaks of a nanosized material. The peaks at 23.7, 39.3 and 46.6°, could be ascribed to (111), (220) and (311) diffraction lines of the face-centered cubic structure of CdTe [33,34]. The narrow peak at 29.5° appearing at a concentration of 2.24 mmol TOP could be attributed to the octahedral phase of Cd3P2 , so testifying the electron diffraction results. It is also observed that Cd3P2 disappeared at the low TOP concentration (Figure 3). The crystal size, as determinated by using the Debye–Scherrer formula, was 3.7 nm, which is in good agree-ment with the value ascertained by TEM. The Debye–Scherrer formula is :
where K is the Scherrer constant, taken as 0.9 for cubic crystal structures, λ is the X-ray wavelength, Δ is the full width at half
maximum (FWHM) of the diffraction peak and θ is the Bragg angle.
Figure 3: X-ray diffraction pattern of deposited CdTe nanocrystals.
Raman spectroscopy is a valuable technique to assess the struc-ture of semiconductors also at the nanometer-scale. In particu-lar, Raman spectroscopy is sensitive to size effects, because like the excitons, phonons experience quantum confinement effects depending on the crystal size. In CdTe, the quantum confine-ment effect is revealed by the broadening and red shifting of the LO mode . Figure 4 shows the cubic CdTe Raman peaks at 142 and 162.3 cm−1 corresponding to TO and LO modes , respectively. It is seen that, the LO mode red-shifts by 5.7 cm−1
with respect to bulk CdTe . On the other hand, all Raman peaks in the range between 200 and 350 cm−1 belong to octahe-dral Cd3P2 , as previously stated by TEM and XRD.
In addition, we have used the Richter–Wang–Law model [37,39], to calculate the crystallite size by fitting the LO peak. The obtained value was 3.4 nm, which is in good agreement with that calculated by TEM and XRD. Interestingly, the CdTe crystallites preserve their size when deposited in the glass sub-strate, so testifying the suitable oleic acid stabilization. In regarding the Cd3P2 formation, it is thought that it was origi-nated by reacting cadmium and phosphor ions, with the latter being provided by the TOP decomposition. Because as reported by Chen et al.  and Henkes et al. , the high reactivity of transition metals promotes the P–C cleavage and the release of the phosphor ions. Surprisingly, the Cd3P2 formation depends on the TOP concentration, because as indicated in Figure 3, for TOP concentration lower than 2.4 mmol, impurity-free CdTe colloids were obtained.
According to Figure 2, our CdTe colloids display a strong red luminescence, indicating quantum confinement in the nano-sized CdTe crystals. It is known that quantum confinement can be observed for crystallite sizes lower than the exciton Bohr radius of the bulk counterpart. In the case of CdTe, the reported parameter is 6.8 nm , whilst the CdTe crystal size was 3.5 nm, as estimated from TEM and XRD measurements. The absorbance spectra shown in Figure 5 exhibit a well-defined peak in the visible wavelength range. This peak corresponds to the band-to-band transition, since it is the most likely transition under the quantum confinement regime . It is worthy to note that CdTe nanocrystals dispersed in toluene showed a narrow absorption peak (or excitonic peak) around 590 nm, suggesting a narrow size distribution for our samples. Neverthe-less the exciton peak disappeared once the CdTe colloid was drop-cast on the glass substrates Figure 5 shows the absorbance spectra of CdTe-NC of the colloidal solution and of a liquid sample processed by the size-separation technique. The effect of size-separation can be observed by considering the maximum absorption peak. The excitonic peak is narrower than that the of the colloid and nearly symmetric, similar to a nearly monodis-persed sample. Additionally, the maximum absorbance has shifted from 607 nm to 589 nm arguing for a lower size disper-sion of the CdTe-NC. However, this result imposes a technolog-ical limitation in the colloid application in a thin-film device due to strong stabilization of oleic acid, which is nonconduc-tive and separates the nanocrystals with spacings of about 0.7 nm and thus impedes their electrical contact .
Oleic acid-stabilized CdTe nanocrystals were prepared by colloidal chemistry. A toluene dispersible product comprising CdTe and Cd3P2 as impurity was obtained. The ink-like disper-sion was successfully to deposit thin films on glass substrate. It
Figure 5: Absorbance spectra of the colloidal solution and CdTe-NC processed by size-separation and re-dispersed in toluene.
was demonstrated that the phase composition depends strongly on the TOP concentration, TOP concentration lower than 2.24 mmol produced free Cd3P2 CdTe colloids.
Materials: cadmium oxide powder ≈1 μm (CdO, 99.5% Aldrich); tellurium powder (200 mesh 99.8% Aldrich); oleic acid (OA, technical grade 90% Aldrich); n-trioctylphosphine (TOP, technical grade 90% Aldrich); 1-octadecene (1-ODC, technical grade 90% Aldrich).
Beilstein J. Nanotechnol.2014,5, 881–886.
Sample preparation to optical and structural characteriza-tion: Initially, the CdTe-NC were processed by a size separa-tion technique. On a colloidal solusepara-tion, ethanol aliquots were dropped and the flocculated solid phase was removed from solution, rinsed also with ethanol and dried with N2. This process was repeated until the solid phase remained completely attached to the flask bottom. Finally, nanocrystals were dispersed with 2–4 mL toluene and deposited on glass substrates via drop-casting technique without annealing. For absorbance characterization, a liquid sample processed by the size-separation technique was analyzed and for Raman measurements, the same sample but deposited by dripping on glass substrate was studied.
TEM characterization: Shape, size and crystal structure of CdTe-NC were determined by transmission electron microscopy (TEM) using a JEOL 2010 microscope. For TEM characterization, the nanocrystals solution were dropped on 300 mesh Lacey carbon grid and dried under laboratory condi-tions. X-ray diffraction (XRD) measurements were done on depositions by using a Bruker AXs D8 Discover diffractometer at normal incidence, using Cu Kα radiation (λ = 0.1506 nm). Absorbance of CdTe colloids and CdTe nanocrystals re-dispersed in toluene were carried out at room temperature by using a Shimadzu 2401 UV–vis spectrophotometer. Raman spectroscopy was carried out also on drop-cast samples by using a Horiba Jobin-Yvon system with an Olympus BX40 microscope, employing the 632 nm He–Ne laser wavelength.
The authors are very thankful to Consejo Nacional de Ciencia y Tecnología (CONACyT-México) by its sponsorship under the grant “2do año de Continuidad de Estancias Posdoctorales Vinculadas al Fortalecimiento de la Calidad del Posgrado Nacional 2013 (2)”. Also, authors are very thankful to Dr. Jaime Santoyo Salazar at the TEM facilities, Álvaro Guzmán Campuzano for his technical assistance in the nanocrystal syn-thesis, and M. Sc. Alejandra García Sotelo for the Raman measurements.
1. Murray, C. B.; Norris, D. J.; Bawendi, M. G. J. Am. Chem. Soc.1993, 115, 8706–8715. doi:10.1021/ja00072a025
2. Murray, C. B.; Kagan, C. R.; Bawendi, M. G. Annu. Rev. Mater. Sci. 2000,30, 545–610. doi:10.1146/annurev.matsci.30.1.545 3. Rogach, A. L.; Franzl, T.; Klar, T. A.; Feldmann, J.; Gaponik, N.;
Lesnyak, V.; Shavel, A.; Eychmüller, A.; Rakovich, Y. P.; Donegan, J. F. J. Phys. Chem. C2007,111, 14628–14637. doi:10.1021/jp072463y
4. Winter, J. O.; Gomez, N.; Gatzert, S.; Schmidt, C. E.; Korgel, B. A.
Colloids Surf., A2005,254, 147–157. doi:10.1016/j.colsurfa.2004.11.024
5. Kumar, A.; Singhal, A. Nanotechnology2007,18, 475703. doi:10.1088/0957-4484/18/47/475703
6. Castro, S. L.; Bailey, S. G.; Raffaelle, R. P.; Banger, K. K.; Hepp, A. F.
J. Phys. Chem. B2004,108, 12429–12435. doi:10.1021/jp049107p 7. Protière, M.; Reiss, P. Small2007,3, 399–403.
8. Zhong, X.; Feng, Y.; Knoll, W.; Han, M. J. Am. Chem. Soc.2003,125,
9. Shavel, A.; Arbiol, J.; Cabot, A. J. Am. Chem. Soc.2010,132,
10. Guo, Q.; Hillhouse, H. W.; Agrawal, R. J. Am. Chem. Soc.2009,131,
11. Talapin, D. V.; Lee, J.-S.; Kovalenko, M. V.; Shevchenko, E. V.
Chem. Rev.2010,110, 389–458. doi:10.1021/cr900137k 12. Bertoni, C.; Gallardo, D.; Dunn, S.; Gaponik, N.; Eychmüller, A.
Appl. Phys. Lett.2007,90, 034107. doi:10.1063/1.2433030 13. Mamedova, N. N.; Kotov, N. A.; Rogach, A. L.; Studer, J. Nano Lett.
2001,1, 281–286. doi:10.1021/nl015519n
14. Lu, W. G.; Fang, J. Y.; Stokes, K. L.; Lin, J. J. Am. Chem. Soc.2004, 126, 11798–11799. doi:10.1021/ja0469131
15. Tang, J.; Kemp, K. W.; Hoogland, S.; Jeong, K. S.; Liu, H.; Levina, L.; Furukawa, M.; Wang, X.; Debnath, R.; Cha, D.; Chou, K. W.; Fischer, A.; Amassian, A.; Asbury, J. B.; Sargent, E. H. Nat. Mater. 2011,10, 765–771. doi:10.1038/nmat3118
16. Luque, J. A.; Martí, A.; Nozik, A. J. MRS Bull.2007,32, 236–241. doi:10.1557/mrs2007.28
17. Peng, S.; Zhang, S.; Mhaisalkar, S. G.; Ramakrishna, S.
Phys. Chem. Chem. Phys.2012,14, 8523–8529. doi:10.1039/c2cp40848a
18. ul Hasan, K.; Nur, O.; Willander, M. Appl. Phys. Lett.2012,100,
19. Tekin, E.; Smith, P. J.; Hoeppener, S.; van den Berg, A. M. J.; Susha, A. S.; Rogach, A. L.; Feldmann, J.; Schubert, U. S.
Adv. Funct. Mater.2007,17, 23–28. doi:10.1002/adfm.200600587 20. Chen, L.; Yang, H.; Qiang, Z.; Pang, H.; Sun, L.; Ma, Z.; Pate, R.;
Stiff-Roberts, A.; Gao, S.; Xu, J.; Brown, G. J.; Zhou, W.
Appl. Phys. Lett.2010,96, 083111. doi:10.1063/1.3337095 21. Urban, J. J.; Talapin, D. V.; Shevchenko, E. V.; Murray, C. B.
J. Am. Chem. Soc.2006,128, 3248–3255. doi:10.1021/ja058269b 22. Hasan, S. A.; Kavich, D. W.; Mahajan, S. V.; Dickerson, J. H.
Thin Solid Films2009,517, 2665–2669. doi:10.1016/j.tsf.2008.10.122 23. Guo, Q.; Kim, S. J.; Kar, M.; Shafarman, W. N.; Birkmire, R. W.;
Stach, E. A.; Agrawal, R.; Hillhouse, H. W. Nano Lett.2008,8,
24. Jasieniak, J.; MacDonald, B. I.; Watkins, S. E.; Mulvaney, P. Nano Lett. 2011,11, 2856–2864. doi:10.1021/nl201282v
25. Sun, X.; Dai, R.; Chen, J.; Zhou, W.; Wang, T.; Kost, A. R.; Tsung, C. K.; An, Z. Opt. Express2014,22, 519–524. doi:10.1364/OE.22.000519
26. de la Presa, P.; Multigner, M.; de la Venta, J.; García, M. A.; Ruiz-González, M. L. J. Appl. Phys.2006,100, 123915. doi:10.1063/1.2401314
27. Vasiliev, R. B.; Vinogradov, V. S.; Dorofeev, S. G.; Kozyrev, S. P.; Kucherenko, I. V.; Novikova, N. N. J. Phys.: Conf. Ser.2007,92,
28. Dzhagan, V.; Lokteva, I.; Himcinschi, C.; Jin, X.; Kolny-Olesiak, J.; Zahn, D. R. T. Nanoscale Res. Lett.2011,6, 79.
29. Haram, S. K.; Kshirsagar, A.; Gujarathi, Y. D.; Ingole, P. P.; Nene, O. A.; Markad, G. B.; Nanavati, S. J. Phys. Chem. C2011,115,
30. Kolny-Olesiak, J.; Kloper, V.; Osovsky, R.; Sashchiuk, A.; Lifshitz, E.
Surf. Sci.2007,601, 2667–2670. doi:10.1016/j.susc.2006.12.013 31. Talapin, D. V.; Haubold, S.; Rogach, A. L.; Kornowski, A.; Haase, M.;
Weller, H. J. Phys. Chem. B2001,105, 2260–2263. doi:10.1021/jp003177o
32. Santoyo-Salazar, J.; Castellanos-Roman, M. A.; Gómez-Looh, B.; Ihiawakrim, D.; Lefevre, C.; Pourroy, G. J. Scanning Probe Microsc. 2009,4, 17–23. doi:10.1166/jspm.2009.1003
33. JCPDS, International Centre for Diffraction Data (PDF 70-8041). 34. Rabadanov, M. K.; Verin, I. A.; Ivanov, Y. M.; Simonov, V. I.
35. Wei, S.; Lu, J.; Yu, W.; Zhang, H.; Qian, Y. Cryst. Growth Des.2006,6,
36. Cullity, B. D. Elements of X-ray Diffraction; Addison–Wesley: Reading, MA, USA, 1956; pp 96–102.
37. Arora, A. K.; Rajalakshmi, M.; Ravindran, T. R. In Encyclopedia of Nanoscience and Nanotechnology; Nalwa, H. S., Ed.; American Scientific Publishers: Valencia, CA, USA, 2004; Vol. 8, pp 499–512. 38. Hellwege, K. H., Ed. Landolt-Bornstein Numerical Data and Functional
Relationships In Science and Technology, New Series, Group III, Vol. 22a and 23a; Springer: Berlin, 1989.
39. Richter, H.; Wang, Z. P.; Ley, L. Solid State Commun.1981,39,
40. Chen, J.-H.; Taib, M.-F.; Chi, K.-M. J. Mater. Chem.2004,14,
41. Henkes, A. E.; Schaak, R. E. Chem. Mater.2007,19, 4235–4242. doi:10.1021/cm071021w
42. Wang, Y.; Zhang, J.; Jia, H.; Li, M.; Zeng, J.; Yang, B.; Zhao, B.; Xu, W.; Lombardi, J. R. J. Phys. Chem. C2008,112, 996–1000. doi:10.1021/jp077467h
43. Huang, Y.; Herron, N. J. Phys. Chem.1991,95, 525–532. doi:10.1021/j100155a009
License and Terms
This is an Open Access article under the terms of the Creative Commons Attribution License
(http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
The license is subject to the Beilstein Journal of Nanotechnology terms and conditions:
The definitive version of this article is the electronic one which can be found at: